Pt Electrodes Enable the Formation of ®¼ O Centers web.mit.edu/dincalab/papers/ Pt...
Embed Size (px)
Transcript of Pt Electrodes Enable the Formation of ®¼ O Centers web.mit.edu/dincalab/papers/ Pt...
Pt Electrodes Enable the Formation of μ4‑O Centers in MOF‑5 from Multiple Oxygen Sources Minyuan M. Li and Mircea Dinca*̆
Department of Chemistry, Massachusetts Institute of Technology, Cambridge, Massachusetts 02139, United States
*S Supporting Information
ABSTRACT: The μ4-O 2− ions in the Zn4O(O2C−)6 secondary building units of
Zn4O(1,4-benzenedicarboxylate)3 (MOF-5) electrodeposited under cathodic bias can be sourced from nitrate, water, and molecular oxygen when using platinum gauze as working electrodes. The use of Zn(ClO4)2·6H2O, anhydrous Zn(NO3)2, or anhydrous Zn(CF3SO3)2 as Zn
2+ sources under rigorous control of other sources of oxygen, including water and O2, confirm that the source of the μ4-O
2− ions can be promiscuous. Although this finding reveals a relatively complicated manifold of electrochemical processes responsible for the crystallization of MOF-5 under cathodic bias, it further highlights the importance of hydroxide intermediates in the formation of the Zn4O(O2C−R) secondary building units in this iconic material and is illustrative of the complicated crystallization mechanisms of metal−organic frameworks in general. KEYWORDS: metal−organic frameworks, electrochemistry, electrodeposition, mechanism of reactions, crystals
Electrode surfaces critically influence the observed potentialof kinetically sluggish redox couples, such as the pH- changing reactions that are commonly used for electrochemi- cally induced crystallizations: water or oxoanion reduction.1 In addition to their electrochemical (i.e., kinetic) influence on the electrodeposition process, electrode surfaces also play key roles in the nucleation and growth of the electrodeposited materials. With this unique offering of controllable variables, electro- deposition becomes an attractive synthetic and mechanistic tool for studying the formation of various crystalline solids.2,3 We have been interested in using electrodeposition to control and study the formation of metal−organic frameworks (MOFs),4−7 whose synthesis is still largely empirical and relies on mechanisms of nucleation and growth that are still poorly understood.8−10
We showed previously that electrochemical reduction of probases such as nitrate (eq 1) on fluorine-doped tin oxide (FTO) leads to the deposition of a thin film of Zn4O(BDC)3 (MOF-5; BDC = 1,4-benzenedicarboxylate; Figure 1).11 Other phases in the Zn-BDC system are also accessible by varying the applied potential, which ultimately affects the identity and activity of various solution species.12 Platinum electrodes are particularly effective for dialing either proton or nitrate reduction events. This allows the modulation of probase at a given potential with concurrent selective crystallization of pure phases and the formation of layered MOF heterostructures by simply dialing the applied potential.13 This unprecedented phase differentiation is important toward utilization of MOFs as functional materials and toward understanding fundamental aspects of solid-phase transformations involved in MOF crystallization. As the use of electrochemical techniques for MOF synthesis receives increasing attention,14−18 mechanistic investigations become critical in guiding future studies. In this work, we further examine the reactivity native to platinum
Special Issue: Hupp 60th Birthday Forum
Received: December 30, 2016 Accepted: February 8, 2017 Published: February 8, 2017
Figure 1. Portion of the crystal structure of MOF-5, highlighting a Zn4O(O2C−)6 cluster. Blue, red, and gray sphere represent Zn, O, and C atoms, respectively. Hydrogen atoms are omitted for clarity.
© XXXX American Chemical Society A DOI: 10.1021/acsami.6b16821 ACS Appl. Mater. Interfaces XXXX, XXX, XXX−XXX
electrodes and show that the source of the μ4-O 2− ions in
MOF-5 is more promiscuous than previously anticipated.
+ + → +− − − −NO H O 2e NO 2OH3 2 2 (1) Despite its iconic status in the field, or perhaps because of it, MOF-5 continues to challenge the fundamental understanding of MOFs. It was recently shown, for instance, that Zn2+ ions dynamically bind solvent molecules and display fast exchange between 4-, 5- and 6-coordination in the as-synthesized material.19 One of the outstanding enigmas related to MOF- 5′s secondary building unit (SBU) is the provenance of the μ4- O2− that bridges the four zinc ions in Zn4O(O2C−)6. Some reports have speculated on the origin of these key bridging ions, surmising that they are products of acid−base reactions involving water,20 by analogy with studies on the formation of molecular basic zinc carboxylate species, Zn4O(O2C−R) (R = alkyl).21,22 A subsequent mechanistic study effected under anhydrous conditions suggested that NO3
− ions were instead the source of μ4-O
2− under solvothermal growth.23 Other reports also showed peroxides facilitating the assembly of Zn4O(O2C−)6 clusters in the presence of triethylamine at room temperature.24,25
+ + → + +− − − −NO H BDC 2e NO H O BDC3 2 2 2 2
We showed previously that NO3 − can function as probase (eq
2) and the sole source of μ4-O 2− in anhydrous N,N-
dimethylformamide (DMF) when using either FTO or Pt as the working electrode (Figure 2 and Figure S1).11,12 This led to
an intriguing question: would MOF-5 form at all in the absence of nitrate? The relevance of this question stems from the fact that MOF-5 crystallization in the presence of nitrate is preceded by the formation of metastable layered zinc hydroxide phases such as Zn5(OH)8(H2O)2·(NO3)2. Because the nitrate anions in these intermediate phases are weakly bound and susceptible to topotactic exchange,12,26 we reasoned that MOF- 5 may indeed be accessible in the absence of nitrate, from a combination of acid−base reactivity between H2BDC and zinc hydroxides (eq 3), and electrochemical generation of HO− by water reduction, for instance (eq 4).
+ → + ‐3H BDC [Zn (OH) ] 7H O MOF 52 4 8 2 (3)
+ → +− −H O e 1 2
H OH2 2 (4)
We performed a series of experiments aimed at eliminating NO3
− from the deposition medium. First, we tested a deposition bath containing no nitrate, with Zn(ClO4)2·6H2O as the source of Zn2+. Applying a potential of −1.50 V (all electrochemical potentials in this work are referenced to the Ag/Ag(cryptand)+ couple, see the Supporting Information) to a Pt gauze electrode in solutions of H2BDC, tetra-n- butylammonium hexafluorophosphate (TBAPF6), and Zn- (ClO4)2·6H2O produced crystalline deposits with weak but well-resolved PXRD peaks corresponding to MOF-5 after 150 min of continuous electrolysis (Figure 3 and Figure S3). In
other words, under conditions where water is the sole source of oxygen atoms, MOF-5 still forms, albeit in lower quantity (Figures S7 and S9). Although perchlorate anions can, in principle, function as probases in a similar manner to nitrate, cyclic voltammetry experiments of tetrabutylammonium perchlorate (TBAP), and H2BDC solutions (i.e., solutions identical to the deposition bath safe for the presence of Zn2+) confirmed that perchlorate is not reduced under these conditions on Pt cathodes (Figures S5 and S6).27 Because we have observed the formation of MOF-5 under cathodic electrolysis in the absence of nitrate, H2O (and HO
−) must be able to act as the sole source for μ4-O
2−. Seeing that H2O is itself a competent probase, we turned our
attention to molecular oxygen, O2, as a potential probase. Under our experimental conditions, we found the O2 reduction potential at approximately −0.70 V (Figure 4), much more anodically shifted than the reduction of Zn2+ to Zn metal. Cyclic voltammetry of an O2-saturated DMF-anh solution indicated one-electron reduction to the superoxide anion radical.28 The large peak-to-peak separation between this event and the oxidation event observed on the reverse potential scan is likely due to adsorption of superoxide onto the Pt electrode surface (eq 5; Ep,c = −1.19 V, Ep,a = −0.42 V).
29,30 In the presence of H2BDC, a new cathodic process is observed at −0.97 V. This likely corresponds to H2 evolution from protons originating either from the carboxylic acid or from O2-derived hydrogen peroxide (eqs 6 and 7).31 Notably, the formation of hydroxide from superoxide or peroxide should be thermody- namically favorable under our deposition potential (eqs 8 and 9).32
Figure 2. PXRD pattern of a sample deposited at −1.50 V on a Pt gauze electrode in DMF-anh with 0.1 M tetra-n-butylammonium hexafluorophosphate (TBAPF6) for 90 min (reagent concentrations: [Zn(NO3)2] = 150 mM, [H2BDC] = 50 mM). The PXRD pattern of MOF-5 is simulated.24 Sample PXRD pattern after isolation in air can be found in Figure S1.
Figure 3. Normalized PXRD patterns of samples deposited at −1.50 V on Pt gauze electrodes in DMF-anh and in DMF-hyd for 150 min (reagent concentrations: [Zn(ClO4)2·6H2O] = 150 mM, [H2BDC] = 50 mM). DMF-hyd is a solution of DMF-anh with 1% v/v of water.
ACS Applied Materials & Interfaces Letter
DOI: 10.1021/acsami.6b16821 ACS Appl. Mater. Interfaces XXXX, XXX, XXX−XXX
http://pubs.acs.org/doi/suppl/10.1021/acsami.6b16821/suppl_file/am6b16821_si_001.pdf http://pubs.acs.org/doi/suppl/10.1021/acsami.6b16821/suppl_file/am6b16821_si_001.pdf http://pubs.acs.org/doi/suppl/10.1021/acsami.6b16821/suppl_file/am6b16821_si_001.pdf http://pubs.acs.org/doi/suppl/10.1021/acsami.6b16821/suppl_file/am6b16821_si_001.pdf http://pubs.acs.org/doi/suppl/10.1021/acsami.6b16821/suppl_file/am6b16821_si_001.pdf http:/